This article needs additional citations for verification. Please help improve this article by adding citations to reliable sources. Unsourced material may be challenged and removed.Find sources: "Stress corrosion cracking" – news · newspapers · books · scholar · JSTOR (December 2007) (Learn how and when to remove this template message)
A close-up of the surface of a steel pipeline showing stress corrosion cracking (two clusters of small black lines) revealed by magnetic particle inspection. Cracks which would normally have been invisible are detectable due to the magnetic particles clustering at the crack openings. The scale at the bottom is in centimeters (each division indicates a millimeter).

Stress corrosion cracking (SCC) is the growth of crack formation in a corrosive environment. It can lead to unexpected and sudden failure of normally ductile metal alloys subjected to a tensile stress, especially at elevated temperature. SCC is highly chemically specific in that certain alloys are likely to undergo SCC only when exposed to a small number of chemical environments. The chemical environment that causes SCC for a given alloy is often one which is only mildly corrosive to the metal. Hence, metal parts with severe SCC can appear bright and shiny, while being filled with microscopic cracks. This factor makes it common for SCC to go undetected prior to failure. SCC often progresses rapidly, and is more common among alloys than pure metals. The specific environment is of crucial importance, and only very small concentrations of certain highly active chemicals are needed to produce catastrophic cracking, often leading to devastating and unexpected failure.[1]

The stresses can be the result of the crevice loads due to stress concentration, or can be caused by the type of assembly or residual stresses from fabrication (e.g. cold working); the residual stresses can be relieved by annealing or other surface treatments. Unexpected and premature failure of chemical process equipment, for example, due to stress corrosion cracking constitutes a serious hazard in terms of safety of personnel, operating facilities and the environment. By weakening the reliability of these types of equipment, such failures also adversely affect productivity and profitability.

## Mechanism

The proposed mechanisms can be classed into two basic categories: anodic mechanisms and cathodic mechanisms. That is, during corrosion, both anodic and cathodic reactions must occur. Also, the phenomena of crack propagation may be associated with either type.[2] For example, the effect of hydrogen on SCC of pipeline steels in the near-neutral pH solutions is often studied. Hydrogen facilitated the dissolution rate of the steel in the solution and increased SCC intensity. A mechanism was proposed that hydrogen enhances the anodic dissolution type of SCC in dilute aqueous solution: hydrogen can diffuse into the steel around the crack tip. Lower pH and lower applied potential facilitate evolution and enrichment of hydrogen during the process of SCC, thus increasing the SCC intensity.[3]

## Material susceptibility

There are several controlling parameters of SCC. The mechanisms that have been proposed for SCC require that certain processes or events occur in sequence for sustained crack propagation to be possible. Therefore, the rate of SCC may be dominated by different reactions. The potential rate-determining steps include:[2]

• Mass transport along the crack to or away from the crack tip
• Reactions in the solution near the crack
• Surface adsorption at or near the crack tip
• Surface diffusion
• Absorption into the bulk
• Bulk diffusion to the plastic zone ahead of the advancing crack

Changes in the environment will dramatically influence the rate of steps above and therefore has an impact on the rate of SCC. Several different environmental parameters are known to influence the rate of crack growth because they influence the reactions above:[2]

### Metals

Alloy KIc

MN/m3/2

SCC environment KIscc

MN/m3/2

13Cr steel 60 3% NaCl 12
18Cr-8Ni 200 42% MgCl2 10
Cu-30Zn 200 NH4OH (pH 7) 1
Al-3Mg-7Zn 25 Aqueous halides 5
Ti-6Al-1V 60 0.6 M KCl 20

With the possible exception of the latter, which is a special example of hydrogen cracking, all the others display the phenomenon of subcritical crack growth, i.e. small surface flaws propagate (usually smoothly) under conditions where fracture mechanics predicts that failure should not occur. That is, in the presence of a corrodent, cracks develop and propagate well below critical stress intensity factor (${\displaystyle K_{\mathrm {Ic} ))$). The subcritical value of the stress intensity, designated as ${\displaystyle K_{\mathrm {Iscc} ))$, may be less than 1% of ${\displaystyle K_{\mathrm {Ic} ))$.

### Polymers

A similar process (environmental stress cracking) occurs in polymers, when products are exposed to specific solvents or aggressive chemicals such as acids and alkalis. As with metals, attack is confined to specific polymers and particular chemicals. Thus polycarbonate is sensitive to attack by alkalis, but not by acids. On the other hand, polyesters are readily degraded by acids, and SCC is a likely failure mechanism. Polymers are susceptible to environmental stress cracking where attacking agents do not necessarily degrade the materials chemically. Nylon is sensitive to degradation by acids, a process known as hydrolysis, and nylon mouldings will crack when attacked by strong acids.

Close-up of broken nylon fuel pipe connector caused by SCC

For example, the fracture surface of a fuel connector showed the progressive growth of the crack from acid attack (Ch) to the final cusp (C) of polymer. In this case the failure was caused by hydrolysis of the polymer by contact with sulfuric acid leaking from a car battery. The degradation reaction is the reverse of the synthesis reaction of the polymer:

Cracks can be formed in many different elastomers by ozone attack, another form of SCC in polymers. Tiny traces of the gas in the air will attack double bonds in rubber chains, with natural rubber, styrene-butadiene rubber, and nitrile butadiene rubber being most sensitive to degradation. Ozone cracks form in products under tension, but the critical strain is very small. The cracks are always oriented at right angles to the strain axis, so will form around the circumference in a rubber tube bent over. Such cracks are dangerous when they occur in fuel pipes because the cracks will grow from the outside exposed surfaces into the bore of the pipe, so fuel leakage and fire may follow. Ozone cracking can be prevented by adding anti-ozonants to the rubber before vulcanization. Ozone cracks were commonly seen in automobile tire sidewalls, but are now seen rarely thanks to the use of these additives. On the other hand, the problem does recur in unprotected products such as rubber tubing and seals.

### Ceramics

This effect is significantly less common in ceramics which are typically more resilient to chemical attack. Although phase changes are common in ceramics under stress these usually result in toughening rather than failure (see Zirconium dioxide). Recent studies have shown that the same driving force for this toughening mechanism can also enhance oxidation of reduced cerium oxide, resulting in slow crack growth and spontaneous failure of dense ceramic bodies.[5]

### Glass

Illustrated are regions of different crack propagation under stress corrosion cracking. In region I, crack propagation is dominated by chemical attack of strained bonds in the crack. In region II, propagation is controlled by diffusion of chemical into the crack. In region III, the stress intensity reaches its critical value and propagates independent of its environment.

Subcritical crack propagation in glasses falls into three regions. In region I, the velocity of crack propagation increases with ambient humidity due to stress-enhanced chemical reaction between the glass and water. In region II, crack propagation velocity is diffusion controlled and dependent on the rate at which chemical reactants can be transported to the tip of the crack. In region III, crack propagation is independent of its environment, having reached a critical stress intensity. Chemicals other than water, like ammonia, can induce subcritical crack propagation in silica glass, but they must have an electron donor site and a proton donor site.[6]

## Prevention

Eliminating that stress, or at least reduce it below the threshold stress for SCC can prevent the SCC. There are methods that can reduce the residual stress.

• For carbon steels, residual stresses can be relieved by stress-relief annealing, and this is also widely used[7]. Carbon steels have the advantage of a relatively high threshold stress for most environments, consequently it is relatively easy to reduce the residual stresses to a low enough level.
• Metallic coatings isolate the metal from the environment and can prevent SCC. For example, zinc is a popular coating for carbon steel. The normal corrosion potential for zinc is relatively low, and the underlying steel is cathodically protected. However, the low electrode potential will also encourage hydrogen evolution and may lead to hydrogen embrittlement.[7]
• Corrosion inhibitors are chemicals that reduce the rate of a corrosive process. However, even when inhibitors are effective against SCC, higher concentrations may be required than for the inhibition of general corrosion. Also, when using inhibitors, notice that chemicals that inhibit general corrosion may accelerate stress corrosion cracking (hydroxides, carbonates and nitrates for carbon steel).[7]
• The compressive residual stresses imparted laser peening are precisely controlled both in location and intensity and can be applied to mitigate sharp transitions into tensile regions. Laser peening imparts deep compressive residual stresses on the order of 10 to 20 times deeper than conventional shot peening, making them significantly more beneficial at preventing SCC.[8] The uniformity with which these processes are applied is important. If only the weld region is shot-peened, damaging tensile stresses may be created at the border of the peened area. Laser peening is widely used in the aerospace and power generation industries in gas fired turbine engines.[9]

## Notable failures

The collapsed Silver Bridge, as seen from the Ohio side
• A 32-inch diameter gas transmission pipeline, north of Natchitoches, Louisiana, belonging to the Tennessee Gas Pipeline exploded and burned from SCC on March 4, 1965, killing 17 people. At least 9 others were injured, and 7 homes 450 feet from the rupture were destroyed.[10][11]
• SCC caused the catastrophic collapse of the Silver Bridge in December 1967, when an eyebar suspension bridge across the Ohio river at Point Pleasant, West Virginia, suddenly failed. The main chain joint failed and the entire structure fell into the river, killing 46 people who were traveling in vehicles across the bridge. Rust in the eyebar joint had caused a stress corrosion crack, which went critical as a result of high bridge loading and low temperature. The failure was exacerbated by a high level of residual stress in the eyebar. The disaster led to a nationwide reappraisal of bridges.[12]

## References

Notes
1. ^ ASM International, Metals Handbook (Desk Edition) Chapter 32 (Failure Analysis), American Society for Metals
2. ^ a b c Jones, R.H. (2017-01-01), Jones, Russell H. (ed.), "Mechanisms of Stress-Corrosion Cracking", Stress-Corrosion Cracking (2 ed.), ASM International, pp. 1–41, doi:10.31399/asm.tb.sccmpe2.t55090001, ISBN 978-1-62708-266-2, retrieved 2022-05-17
3. ^ Gu, B.; Luo, J.; Mao, X. (January 1999). "Hydrogen-Facilitated Anodic Dissolution-Type Stress Corrosion Cracking of Pipeline Steels in Near-Neutral pH Solution". CORROSION. 55 (1): 96–106. doi:10.5006/1.3283971. ISSN 0010-9312.
4. ^ Baker, H. R.; Bloom, M. C.; Bolster, R. N.; Singleterry, C. R. (1970-09-01). "Film and pH Effects in the Stress Corrosion Cracking of Type 304 Stainless Steel". Corrosion. 26 (10): 420–426. doi:10.5006/0010-9312-26.10.420. ISSN 1938-159X.
5. ^ Munnings, C.; Badwal, S. P. S.; Fini, D. (20 February 2014). "Spontaneous stress-induced oxidation of Ce ions in Gd-doped ceria at room temperature". Ionics. 20 (8): 1117–1126. doi:10.1007/s11581-014-1079-2. S2CID 95469920.
6. ^ Wachtman, John B.; Cannon, W. Roger; Matthewson, M. John (11 September 2009). Mechanical Properties of Ceramics (2nd ed.). John Wiley and Sons. doi:10.1002/9780470451519. ISBN 9780471735816.
7. ^ a b c "Controlling stress corrosion cracking". corrosion-doctors.org. Retrieved 2022-05-18.
8. ^ EPRI | Search Results: Compressor Dependability: Laser Shock Peening Surface Treatment
9. ^
10. ^
11. ^ The Washington Observer - Google News Archive Search
12. ^ Lewis, Peter Rhys, Reynolds, K, and Gagg, C, Forensic Materials Engineering: Case studies, CRC Press (2004).
Sources
• ASM International, Metals Handbook (Desk Edition) Chapter 32 (Failure Analysis), American Society for Metals, (1997) pp 32–24 to 32-26
• ASM Handbook Volume 11 "Failure Analysis and Prevention" (2002) "Stress-Corrosion Cracking" Revised by W.R. Warke, American Society of Metals. Pages 1738-1820
• "Mechanical Properties of Ceramics" by John B. Wachtman, W. Roger Cannon, and M. John Matthewson. Chapter 8.